Periodic table (crystal structure)

For elements that are solid at standard temperature and pressure the table gives the crystalline structure of the most thermodynamically stable form(s) in those conditions. In all other cases the structure given is for the element at its melting point (H, He, N, O, F, Ne, Cl, Ar, Kr, Xe, and Rn are gases at STP; Br, Hg, and probably Cn and Fl are liquids at STP). Predictions are given for At, Fr, elements 100–113 and 118, which have not been produced in bulk. The latest predictions for Fl (element 114) could not distinguish between face-centred cubic and hexagonal close-packed structures, which were predicted to be close in energy.[1] No predictions are available for elements 115–117.

## Contents

* 1 Table
* 2 Unusual structures
* 3 Usual crystal structures
* 3.1 Close packed metal structures
* 3.1.1 Hexagonal close packed
* 3.1.2 Face-centered cubic (cubic close packed)
* 3.1.3 Double hexagonal close packed
* 3.2 Body centred cubic
* 4 See also
* 5 References
* 6 External links

## Table

## Unusual structures

Element | crystal system | coordination number | notes

|
|
|

Mn | cubic | distorted bcc – unit cell contains Mn atoms in 4 different environments.[2] |
Zn | hexagonal | distorted from ideal hcp. 6 nearest neighbors in same plane: 6 in adjacent planes 14% farther away[2] |
Ga | orthorhombic | each Ga atom has one nearest neighbour at 244 pm, 2 at 270 pm, 2 at 273 pm, 2 at 279 pm.[2] | The structure is related to that of iodine.
As | rhombohedral | puckered sheet; each As atom has 3 neighbours in the same sheet at 251.7pm; 3 in adjacent sheet at 312.0 pm.[2] | grey metallic form.
Cd | hexagonal | distorted from ideal hcp. 6 nearest neighbours in the same plane- 6 in adjacent planes 15% farther away[2] |
In | tetragonal | slightly distorted fcc structure[2] |
Sn | tetragonal | 4 neighbours at 302 pm; 2 at 318 pm; 4 at 377 pm; 8 at 441 pm [2] | white tin form (thermodynamical stable above 286.4 K)
Sb | rhombohedral | puckered sheet; each Sb atom has 3 neighbours in the same sheet at 290.8pm; 3 in adjacent sheet at 335.5 pm.[2] | grey metallic form.
Sm | trigonal | 12 nearest neighbours | complex hcp with 9-layer repeat: ABCBCACAB....[3]
Hg | rhombohedral | 6 nearest neighbours at 234 K and 1 atm (it is liquid at room temperature and thus has no crystal structure at ambient conditions!) | this structure can be considered to be a distorted hcp lattice with the nearest neighbours in the same plane being approx 16% farther away [2]
Bi | rhombohedral | puckered sheet; each Bi atom has 3 neighbours in the same sheet at 307.2 pm; 3 in adjacent sheet at 352.9 pm.[2] | Bi, Sb and grey As have the same space group in their crystal
Po | cubic | 6 nearest neighbours | simple cubic lattice. The atoms in the unit cell are at the corner of a cube.
Pa | tetragonal | body centred tetragonal unit cell, which can be considered to be a distorted bcc |
U | orthorhombic | strongly distorted hcp structure. Each atom has four near neighbours, 2 at 275.4 pm, 2 at 285.4 pm. The next four at distances 326.3 pm and four more at 334.2 pm.[4] |
Np | orthorhombic | highly distorted bcc structure. Lattice parameters: a = 666.3 pm, b = 472.3 pm, c = 488.7 pm [5][6] |
Pu | monoclinic | slightly distorted hexagonal structure. 16 atoms per unit cell. Lattice parameters: a = 618.3 pm, b = 482.2 pm, c = 1096.3 pm, β = 101.79° [7][8] |

## Usual crystal structures

### Close packed metal structures

Many metals adopt close packed structures i.e. hexagonal close packed and face-centred cubic structures (cubic close packed). A simple model for both of these is to assume that the metal atoms are spherical and are packed together in the most efficient way (close packing or closest packing). In closest packing every atom has 12 equidistant nearest neighbours, and therefore a coordination number of 12. If the close packed structures are considered as being built of layers of spheres then the difference between hexagonal close packing and face-centred cubic is how each layer is positioned relative to others. Whilst there are many ways that can be envisaged for a regular buildup of layers:

* hexagonal close packing has alternate layers positioned directly above/below each other: A,B,A,B,... (also termed P63/mmc, Pearson symbol hP2, strukturbericht A3) .
* face-centered cubic has every third layer directly above/below each other: A,B,C,A,B,C,... (also termed cubic close packing, Fm3m, Pearson symbol cF4, strukturbericht A1) .
* double hexagonal close packing has layers directly above/below each other, A,B,A,C,A,B,A,C,.... of period length 4 like an alternative mixture of fcc and hcp packing (also termed P63/mmc, Pearson Symbol hP4, strukturbericht A3' ).[9]
* α-Sm packing has a period of 9 layers A,B,A,B,C,B,C,A,C,.... (R3m, Pearson Symbol hR3, strukturbericht C19).[10]

#### Hexagonal close packed

In the ideal hcp structure the unit cell axial ratio is [math]\displaystyle{ 2\sqrt{\frac{2}{3}} \sim 1.633 }[/math]. However, there are deviations from this in some metals where the unit cell is distorted in one direction but the structure still retains the hcp space group—remarkable all the elements have a ratio of lattice parameters c/a < 1.633 (best are Mg and Co and worst Be with c/a ~ 1.568). In others like Zn and Cd the deviations from the ideal change the symmetry of the structure and these have a lattice parameter ratio c/a > 1.85.

#### Face-centered cubic (cubic close packed)

More content relating to number of planes within structure and implications for glide/slide e.g. ductility.

#### Double hexagonal close packed

Similar to the ideal hcp structure, the perfect dhcp structure should have a lattice parameter ratio of [math]\displaystyle{ \frac{c}{a} = 4\sqrt{\frac{2}{3}} \sim 3.267. }[/math] In the real dhcp structures of 5 lanthanides (including β-Ce) [math]\displaystyle{ c/2a }[/math] variates between 1.596 (Pm) and 1.6128 (Nd). For the four known actinides dhcp lattices the corresponding number vary between 1.620 (Bk) and 1.625 (Cf).[11]

### Body centred cubic

This is not a close packed structure. In this each metal atom is at the centre of a cube with 8 nearest neighbors, however the 6 atoms at the centres of the adjacent cubes are only approximately 15% further away so the coordination number can therefore be considered to be 14 when these are ong one 4 fold axe structure becomes face-centred cubic (cubic close packed).

## See also

* Crystal structure

## References

1. ↑ Florez, Edison; Smits, Odile R.; Mewes, Jan-Michael; Jerabek, Paul; Schwerdtfeger, Peter (2022). "From the gas phase to the solid state: The chemical bonding in the superheavy element flerovium". The Journal of Chemical Physics 157. doi:10.1063/5.0097642.
2. ↑ 2.0 2.1 2.2 2.3 2.4 2.5 2.6 2.7 2.8 2.9 Greenwood, Norman N.; Earnshaw, Alan (1997). Chemistry of the Elements (2nd ed.). Butterworth-Heinemann. ISBN 978-0-08-037941-8.
3. ↑ A.F Wells (1962) Structural Inorganic Chemistry 3d Edition Oxford University Press
4. ↑ Harry L. Yakel, A REVIEW OF X-RAY DIFFRACTION STUDIES IN URANIUM ALLOYS. The Physical Metallurgy of Uranium Alloys Conference, Vail, Colorado, Feb. 1974
5. ↑ Lemire, R.J. et al.,Chemical Thermodynamics of Neptunium and Plutonium, Elsevier, Amsterdam, 2001
6. ↑ URL "The alpha Np (A_c) Structure". http://cst-www.nrl.navy.mil/lattice/struk/a_c.html.
7. ↑ Lemire, R. J. et al.,2001
8. ↑ URL "The alpha-Pu Structure". http://cst-www.nrl.navy.mil/lattice/struk/aPu.html.
9. ↑ URL "The alpha la (A3') Structure". http://cst-www.nrl.navy.mil/lattice/struk/a3p.html.
10. ↑ URL "The alpha Sm (C19) Structure". http://cst-www.nrl.navy.mil/lattice/struk/c19.html.
11. ↑ Nevill Gonalez Swacki & Teresa Swacka, Basic elements of Crystallography, Pan Standford Publishing Pte. Ltd., 2010

General

* "Actinides and the Environment". NATO ASI Series. Maleme, Crete, Greece: Kluver Academic Publishers. July 1996. pp. 59–61. ISBN 0-7923-4968-7.
* The Chemistry of the Actinide and Transactinide Elements (3rd ed.). Springer. 2007. ISBN 978-1402035555.

## External links

* Strukturbericht Type A – structure reports for the pure elements
* Crystal Structures for the solid chemical elements at 1 bar

* v
* t
* e

Periodic table

Periodic table forms|

| Standard|

* 18-column
* 32-column

|

Alternative|

* Alternatives
* Janet's left step table

Extended|

* Extension beyond the 7th period
* Aufbau
* Fricke
* Pyykkö

Sets of elements|

| By periodic table structure|

| Groups|

* 1 (Alkali metals)
* 2 (Alkaline earth metals)
* 3
* 4
* 5
* 6
* 7
* 8
* 9
* 10
* 11
* 12
* 13
* 14
* 15 (Pnictogens)
* 16 (Chalcogens)
* 17 (Halogens)
* 18 (Noble gases)

|

Periods|

* 1
* 2
* 3
* 4
* 5
* 6
* 7
* 8+
* Aufbau
* Fricke
* Pyykkö

Blocks|

* s-block
* p-block
* d-block
* f-block
* g-block
* Aufbau principle

By metallicity|

| Metals|

* Alkali metals
* Alkaline earth metals
* Lanthanides
* Actinides
* Transition metals
* Post-transition metals

|

Metalloids|

* Lists of metalloids by source
* Dividing line

Nonmetals|

* Reactive nonmetals
* Noble gases

Other sets|

* Platinum-group metals (PGM)
* Rare-earth elements
* Refractory metals
* Precious metals
* Coinage metals
* Noble metal
* Heavy metals
* Native metals
* Transuranium elements
* Superheavy elements
* Major actinides
* Minor actinides

Elements|

| Lists|

* By: Abundance (in humans)
* Atomic properties
* Nuclear stability
* Production
* Symbol

|

Properties|

* Crystal structure
* Electron configuration
* Electronegativity
* Goldschmidt classification
* Term symbol

Data pages|

* Abundance
* Atomic radius
* Boiling point
* Critical point
* Density
* Elasticity
* Electrical resistivity
* Electron affinity
* Electron configuration
* Electronegativity
* Hardness
* Heat capacity
* Heat of fusion
* Heat of vaporization
* Ionization energy
* Melting point
* Oxidation state
* Speed of sound
* Thermal conductivity
* Thermal expansion coefficient
* Vapor pressure

History|

* Element discoveries
* Mendeleev's predictions
* Naming
* etymology
* controversies
* for places
* for people
* in East Asia

See also|

* IUPAC
* nomenclature
* systematic element name
* Trivial name
* Dmitri Mendeleev

* Book
* Category

0.00

(0 votes)

Original source: https://en.wikipedia.org/wiki/Periodic table (crystal structure). Read more

|

Retrieved from "https://handwiki.org/wiki/index.php?title=Chemistry:Periodic_table_(crystal_structure)&oldid=2596350"
*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template